Direct-writing of PbS nanoparticles inside transparent porous silica monoliths using pulsed femtosecond laser irradiation
© Chahadih et al; licensee Springer. 2011
Received: 27 June 2011
Accepted: 4 October 2011
Published: 4 October 2011
Pulsed femtosecond laser irradiation at low repetition rate, without any annealing, has been used to localize the growth of PbS nanoparticles, for the first time, inside a transparent porous silica matrix prepared by a sol-gel route. Before the irradiation, the porous silica host has been soaked within a solution containing PbS precursors. The effect of the incident laser power on the particle size was studied. X-ray diffraction was used to identify the PbS crystallites inside the irradiated areas and to estimate the average particle size. The localized laser irradiation led to PbS crystallite size ranging between 4 and 8 nm, depending on the incident femtosecond laser power. The optical properties of the obtained PbS-silica nanocomposites have been investigated using absorption and photoluminescence spectroscopies. Finally, the stability of PbS nanoparticles embedded inside the host matrices has been followed as a function of time, and it has been shown that this stability depends on the nanoparticle mean size.
New directions of modern research have emerged during the last decade, which has broadly been defined as nanoscale science and technology [1, 2]. These new trends involve the ability to fabricate, characterize, and manipulate artificial structures, the features of which are controlled at the nanometer scale. The semiconductor properties of lead sulfide PbS have widely been used in elements such as detectors operating in the infra-red spectral region (from 850 to 3100 nm) , solar batteries , and advanced optoelectronic devices . In most of recent applications, useful properties of the PbS nanoparticles arise from the strong quantum confinement effect of the charge carriers (Bohr radius of 18 nm) and the associated optical nonlinear property .
Semiconductors may be included in a variety of media including polymers [7–9], micelles [10, 11], glassy particles , and zeolites . The synthesis of semiconducting nanoparticles in glass matrices has become very important. A number of methods to synthesize semiconductor nano-crystals have been employed and these include hydrothermal synthesis , chemical bath , spray pyrolysis , laser-heated evaporation , combustion synthesis , and the sol-gel technique . The sol-gel technique has become very popular because of the high chemical homogeneity of the products, also to the low processing temperatures, the possibility of controlling the particles size and morphology. The sol-gel-derived materials provide excellent matrices for a variety of organic and inorganic compounds. Silica porous matrices can be obtained using the sol-gel process and depending on how the wet gel is dried, the porosity of the materials can be tailored . Such a controlled porosity can be used to dope it with active elements by impregnation with appropriate solutions.
A few articles have been reported in the literature on the crystallization of PbS nanoparticles by heat-treatment inside a silica matrix prepared by sol-gel method [21–23]. In this case, however, the precipitation of semiconductor nanoparticles has been realized without any space-localization. To reach this aim, the use of a laser irradiation is a promising method. Recently, local precipitation of PbS nanoparticles in melting glass matrix has been reported [24, 25]. Chao et al.  used pulsed femtosecond laser irradiation (800 nm, 1 kHz, and 184 fs) followed by a heat treatment at a temperature of 450°C to precipitate PbS nanoparticles inside irradiated areas of a melted glass. Takeshima et al.  reported the local precipitation of PbS inside a melted glass without annealing using a pulsed femtosecond laser irradiation at high repetition rate (250 kHz, 200 fs, 750 mW). Recently, we have reported the space-selective growth of CdS nanoparticles, at ambient conditions, inside silica xerogels by laser irradiation .
Herein, we report on our investigations, based on a pulsed femtosecond laser irradiation performed with a low repetition rate in ambient conditions, for the localized growth of PbS nanoparticles inside a deep volume of porous silica monoliths. Moreover, we provide a study on the stability of PbS nanoparticles as a function of time.
Porous silica xerogels with a thickness of 2 mm has been prepared by a sol-gel route using tetramethylorthosilicate . The obtained silica monolith exhibited interconnected pores of mean diameter 5.4 nm, a specific surface area of 360 m2 g-1 and a pore volume of 0.49 cm3 g-1. All these parameters were determined by isothermal nitrogen sorption measurements, as previously described . The obtained porous silica samples were impregnated for 4 h into an aqueous solution (S) composed of the lead acetate as a lead precursor and of thiourea as a sulfur precursor. The concentration of each precursor in S was 0.37 mol L-1 and the molar ratio between Pb and S sources was kept to 1.
Absorption spectra were recorded at room temperature in the irradiated zone using a Perkin-Elmer lambda 19 UV-Vis-IR double beam spectrometer.
Micro-photoluminescence measurements have been performed using a HORIBA Jobin Yvon IHR320 spectrometer coupled with a microscope at room temperature. Both 351.1 and 514.5 nm laser lines of an argon laser have been used to excite the PbS-doped silica matrices in the fs-irradiated zone. The incident laser power was kept low enough to avoid any further precipitation of PbS nanoparticles.
XRD patterns are recorded on a Philips X'Pert diffractometer equipped with a monochromator, using Cu Kα radiation.
TEM characterization was performed on a microscope FEI Tecnai G2-20 twin with a 200 kV acceleration voltage. For TEM imaging, the precipitated zone of a doped sample was grinded into a powder and then deposited onto a copper grid previously coated with a thin carbon membrane. The powder was then metalized with a vaporized carbon layer.
Result and discussion
The irradiation wavelength 800 nm corresponds to energy much smaller than the band gap of silica. Hence, no linear absorption can occur when the matrix is irradiated, thus allowing the laser beam to penetrate deeply inside the material. Hence, it is possible to embed a PbS layer of nanoparticles anywhere in the monolith. However, even at the lowest average power corresponding to tremendous laser peak power, a multi-photon absorption exists. As a result, the impact area is highly localized, confined within the focal volume of the focused beam. The irradiated zone showed brown or black color, depending on the average power of the laser beam. This color is easily visible to the naked eye, as shown in Figure 1.
The formation of PbS nanocrystals inside the porous silica glass, after laser irradiation, was confirmed by different analysis techniques. According to the different analysis techniques, we have irradiated at different depths: just under the surface for XRD measurements and for the other characterisations, the focused beam was in the middle of the monolith.
Photoluminescence spectra of the area irradiated with a power of 40 mW and in the unirradiated area are shown in Figure 3(right). Under excitation with the 351 nm laser line, the non-irradiated area emits light in a large band centered on 600 nm, while the excitation of the irradiated area at the same wavelength results in two emission bands: the first one being centered on 650 nm and the second one around 910 nm. Consequently, the bands peaking at 600 and 650 nm could be attributed to the luminescence of PbS precursors and SiO2 host matrix, since the S-doped silica absorption at 350 nm is still strong. On the other hand, the PL band centered at 910 nm is due to the PbS nanoparticles. To confirm our assumption, the same PL spectra were recorded under excitation at 514.5 nm. At this wavelength, the S-loaded matrix absorbs less and as a result, no emission could be observed in the non-irradiated area. However, in the case of the irradiated area, both emission bands are still present, although red-shifted by 20 nm. As far as the PbS nanoparticles are concerned, the red-shift of the 650 nm emission band can be interpreted through a resonant size-selection by the excitation wavelength, as already observed with CdS particles . The same kind of selection process in the electronic level population may be assumed for the "matrix band" at 650 nm. Meanwhile, the intensity ratio between these two emission bands is inverted when switching from UV to visible excitation. This can easily be understood as the result of a drastic decreasing number of absorbing entities in the non-irradiated zone between 351 and 514 nm wavelengths. The maximum of the emission band located around 930 nm is because of the presence of dominant small PbS nanoparticles (3-5 nm) . This maximum emission is shifted toward lower wavelengths comparing to the one reported by Hines and Scholes  for a bigger colloidal PbS with a size of 6.5 nm.
In the literature, the mechanism of PbS nanoparticles formation inside a porous silica matrix has been explained by pyrolysis or decomposition of the PbS precursor under heat treatment [21, 22]. Moreover, Chao et al.  have reported on the mechanism of PbS nanoparticles precipitation inside melting glasses induced by a femtosecond laser: when glasses containing lead and sulfur are submitted to a femtosecond laser irradiation, it can probably induce ion-exchange effects and a redistribution of network modifiers, resulting in the enrichment of the laser-irradiated zone in lead and sulfur atoms. This enrichment makes it possible to decrease the thermal treatment temperature. Hence, the formation of bigger and denser quantum dots in the irradiated area is accelerated after a subsequent and necessary heat treatment. In our case, the nano-crystallization of PbS inside the porous silica occurred in the region of the laser irradiation without any further annealing because of two main processes. First, the multi-photon absorption of the porous silica matrix and of the PbS precursors at 800 nm  leads to the decomposition of these precursors, thus enriching the irradiated zone with lead and sulfur ions. In the same time, the temperature elevation during the laser pulse could be sufficient to aggregate the molecular PbS into nanoparticles [26, 31].
Calculated sizes of PbS nanoparticles from XRD measurements for different laser average powers
Sizes calculated from XRD (nm)
The most important drawback that limits the use of PbS nanoparticles in many applications is their low chemical stability. This is due to their high ability to oxidation, which limits their use under ambient conditions.
These preliminary results demonstrate that the stability of PbS nanoparticles, inside the porous host matrix, depends on their size. It should be recalled that the PbS particle mean size, as deduced from the XRD measurements around time t0, has been evaluated to 4 and 8 nm after irradiations with 10 and 40 mW, respectively (see Table 1). In the first case, the crystallite size is thus lower than the average matrix pore size of 5.4 nm, as opposed to the case of 40 mW irradiation. Since the diameter size of PbS nanoparticles created with 40 mW is greater than the pore diameter, it implies that, under the extreme local conditions of the femtosecond laser-induced plasma, the created nanoparticles are capable of breaking the walls of the interconnected pores during their formation. An important amount of oxygen is then allowed to diffuse inside the matrix and to react with PbS nanoparticles, leading to their oxidation in several days. It has been noticed that the oxidation rate seems to decrease versus time. This shift in the absorption band edge could be explained by the formation of core-shell structure with unknown shell phase. Indeed several oxide phases can be observed when PbS is oxidized such as PbO. PbSO4 . We have already detected this phase when we irradiate the doped monoliths by 514.5 nm continuous laser. On the contrary, no oxidation was observed with a lower laser power of 10 mW, but most of the nanoparticles have a size (4 nm) suited to the pores. In this case, it is likely that the nanoparticles have grown without any modification of the silica matrix and these particles remain protected from oxidation by the silica walls. This effect could explain the stability of PbS nanoparticles, even after 100 days. Hence, both the pore diameter of the host silica matrix and the power of pulsed femtosecond laser irradiation play an important role in the stability of the obtained PbS nanoparticles.
The formation of PbS nanoparticles localized inside porous silica xerogels has been performed using the pulsed femtosecond laser irradiation without any annealing. Characterization of the obtained nanocrystals was allowed by writing a tight network of PbS lines in a centimeter-sized zone near the surface or in the depth of the bulk xerogel. Most of the crystallites have been identified as cubic phase of PbS by XRD and TEM. We have shown that the power laser can be used to control the mean particle size between 4 and 8 nm. The micro-PL data made it possible to identify an emission band coming from the matrix and PbS precursors, and another band assigned to PbS nanoparticles, which are resonantly wavelength-selected in size. Finally, the stability of PbS nanoparticles under ambient conditions depends on the particle size, monitored by the laser power, and on the porosity of the host matrix.
This study was supported by the French Agence Nationale de la Recherche (ANR) in the frame of the POMESCO project (Organized Photo-growth of Metallic and Semi-Conductor Nano-Objects Intended to Optic Devices), the "Conseil Régional Nord Pas de Calais Picardie" and the "Fonds Européen de Développement Economique des Régions".
- Lane N: The grand challenges of nanotechnology. J Nanopart Res 2001, 3: 95–103. 10.1023/A:1017951230941View ArticleGoogle Scholar
- Service RF: Is nanotechnology dangerous? Science 2000, 290: 1526.View ArticleGoogle Scholar
- Masek J, Ishida A, Zogg H: Monolithic photovoltaic PbS-on-Si infrared-sensor array. IEEE Electron Dev Lett 1990, 11: 12–14. 10.1109/55.46915View ArticleGoogle Scholar
- Serap G, Karolina PF, Helmut N, Niyazi S, Sandeep K, Gregory DS: Hybrid solar cells using PbS nanoparticles. Sol Energy Mater Sol Cells 2007, 91: 420–423. 10.1016/j.solmat.2006.10.016View ArticleGoogle Scholar
- Asunskis D, Bolotin I, Wroble A, Zachary A, Hanley L: Lead sulfide nanocrystal-polymer composites for optoelectronic applications. Macromol Symp 2008, 268: 33–37. 10.1002/masy.200850807View ArticleGoogle Scholar
- Dan L, Chunjun L, Yw L, Shixiong Q: Femtosecond nonlinear optical properties of PbS nanoparticles. J Lumin 2007, 122: 549–551.Google Scholar
- Kuczski J, Milosaljevic B, Thomas J: Photophysical properties of cadmium sulfide in nafion film. J Phys Chem 1984, 88: 980–984. 10.1021/j150649a027View ArticleGoogle Scholar
- Meisser D, Memming R, Kastening B: Light-induced generation of hydrogen at CdS-monograin membranes. Chem Phys Lett 1983, 96: 34. 10.1016/0009-2614(83)80112-2View ArticleGoogle Scholar
- Wang Y, Suna A, Mahler W, Kawasaki R: PbS in polymer: from molecules to bulk solids. J Chem Phys 1987, 87: 7315. 10.1063/1.453325View ArticleGoogle Scholar
- Tricot Y, Fendler J: In situ generated colloidal semiconductor CdS particles in dihexadecyl phosphate vesicles: quantum size and asymmetry effects. J Phys Chem 1986, 90: 3369–3374. 10.1021/j100406a013View ArticleGoogle Scholar
- Wartzke H, Fendler J: Quantum size effects of in situ generated colloidal CdS particles in dioctadecyldimethylammonium chloride surfactant vesicles. J Phys Chem 1987, 91: 854–861. 10.1021/j100288a019View ArticleGoogle Scholar
- Kuczski J, Thomas J: Photophysical properties of cadmium sulfide deposited in porous vycor glass. J Phys Chem 1985, 89: 2720–2722. 10.1021/j100259a002View ArticleGoogle Scholar
- Wang Y, Herron N: Optical properties of CdS and PbS clusters encapsulated in zeolites. J Phys Chem 1987, 91: 257–260. 10.1021/j100286a004View ArticleGoogle Scholar
- Yang Y, He L, Zhang Q: A cyclic voltametric synthesis of PbS nanoparticles. Electrochem Commun 2005, 7: 361–364. 10.1016/j.elecom.2005.02.005View ArticleGoogle Scholar
- Patil R, Lokhande C, Mane R, Gujar T, Han S: Room temperature PbS nanoparticle growth, incubation in porous TiO 2 electrode for photosensitization application. J Noncryst Solids 2007, 353: 1645–1649. 10.1016/j.jnoncrysol.2007.01.014View ArticleGoogle Scholar
- Sha L, Wang Z, Mark T: Spray pyrolysis synthesis of ZnS nanoparticles from a single-source precursor. Nanotechnology 2009, 20: 235603. 10.1088/0957-4484/20/23/235603View ArticleGoogle Scholar
- Musikhiin S, Bakueva L, Rabizo O, Rykov S: Quantum-size layered PbS/C structures deposited by pulsed laser evaporation in vacuum. Mater Sci Eng B 1995, 35: 120–124. 10.1016/0921-5107(95)01409-8View ArticleGoogle Scholar
- Swihart M: Vapor-phase synthesis of nanoparticles. Curr Opin Colloid Interface Sci 2003, 8: 127–133. 10.1016/S1359-0294(03)00007-4View ArticleGoogle Scholar
- Capoen B, Martucci A, Turrell S, Bouazaoui M: Effects of the sol-gel solution host on the chemical and optical properties of PbS quantum dots. J Mol Struct 2003, 651–653: 467–473.View ArticleGoogle Scholar
- El Hamzaoui H, Courthéoux L, Nguyen V, Berrier V, Favre A, Bigot L, Bouazaoui M, Capoen B: From porous silica xerogels to bulk optical glasses: the control of densification. Mater Chem Phys 2010, 121: 83–88. 10.1016/j.matchemphys.2009.12.043View ArticleGoogle Scholar
- Parvathy N, Pajonk G, Rao A: Effects of temperature and sol-gel parameters on PbS crystallite sizes and their spectral and physical properties in a porous silica matrix. J Noncryst Solids 1998, 241: 79–90. 10.1016/S0022-3093(98)00768-6View ArticleGoogle Scholar
- Parvathy N, Pajonk G, Rao A: Processing and characterisation of PbS nano-crystallites in TMOS silica xerogel. Mater Res Bull 1997, 32: 397–408. 10.1016/S0025-5408(97)00004-4View ArticleGoogle Scholar
- Dementjev A, Gulbinas V: Excited state absorption of PbS nanocrystals in silicate glass. Opt Mater 2009, 31: 647–652. 10.1016/j.optmat.2008.07.002View ArticleGoogle Scholar
- Chao L, Yong K, Jong H: Controlled precipitation of lead sulfide quantum dots in glasses using the femtosecond laser pulses. J Am Ceram Soc 2010, 93: 1221–1224.View ArticleGoogle Scholar
- Nobuhito T, Yutaka K, Yoshihiro N, Shuhei T: Fabrication of a periodic structure with a high refractive-index difference by femtosecond laser pulses. Opt Express 2004, 12: 4020–4024.Google Scholar
- El Hamzaoui H, Bernard R, Chahadih A, Chassagneux F, Bois L, Jegouso D, Hay L, Capoen B, Bouazaoui M: Laser-induced direct space-selective precipitation of CdS nanoparticles embedded in a transparent silica xerogel. Nanotechnology 2010, 21: 134002. 10.1088/0957-4484/21/13/134002View ArticleGoogle Scholar
- Capoen B, Gacoin T, Nedelec JM, Turrell S, Bouazaoui M: Spectroscopic investigations of CdS nanoparticles in sol-gel derived polymeric thin films and bulk silica matrices. J Mater Sci 2001, 36: 2565–2570. 10.1023/A:1017958821681View ArticleGoogle Scholar
- Chao L, Yong K, Jong H: Absorption and photoluminescence of PbS QDs in glasses. J Noncryst Solids 2009, 355: 1880–1883. 10.1016/j.jnoncrysol.2009.04.045View ArticleGoogle Scholar
- Hines M, Scholes G: Colloïdal PbS nanocrystals with size-tunable near-infrared emission: observation of post synthesis self-narrowing of the particle size distribution. Adv Mater 2003, 15: 1844–1849. 10.1002/adma.200305395View ArticleGoogle Scholar
- Raulin K, Cristini O, Baldeck P, Stéphane O, Kinowski C, Turelle S, Capoen B, Bouazaoui M: A novel femtosecond-laser formation of CdS nanocrystallites in zirconia matrices. J Nanopart Res 2010, 12: 1459–1467. 10.1007/s11051-009-9715-xView ArticleGoogle Scholar
- El Hamzaoui H, Bernard R, Chahadih A, Chassagneux F, Bois L, Jegouso D, Hay L, Capoen B, Bouazaoui M: Room temperature direct space-selective growth of gold nanoparticles inside a silica matrix based on a femtosecond laser irradiation. Mater Lett 2010, 64: 1279–1282. 10.1016/j.matlet.2010.03.008View ArticleGoogle Scholar
- Cullity B: Elements of X-Ray Diffraction. 2nd edition. Wiley; 1978.Google Scholar
- Sadovnikov SI, Kozhevnikova NS, Rempel AA: Stability and recrystallization of PbS nanoparticle. Inorg Mater 2011, 47: 837–843. 10.1134/S0020168511080176View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.